Fig.4.1 shows the overall structure of the hybrid laser. As explained in Chapter 2, although the scattering loss increases, a structure in which epitaxy is terminated at both ends of the mirror is adopted abruptly for single mode operation. The part with the mirror within silicon waveguide is indicated by a black dash line. The area marked in orange and yellow is the III-V gain section, the dark gray is the Si device layer, and the light gray is the BOX layer. Yellow is the metal for ohmic contact, the top and bottom are n-ohmic metal, and the middle is p-ohmic metal. The parts overlapping the two regions of the p(n) metal pad and the n(p) ohmic metal were separated using Photo-BCB (cyclotene 4022-35). For an efficient heat dissipation structure, the metal pad is thickly deposited.
Figure 4.1: Schematic of hybrid in-plane laser
Schematic of process flow
Figure 4.2: process flow of hybrid in-plane laser.
Fig.4.2 shows the processes required to make a hybrid laser. Because of the limited quantity and high price of III-V wafers, all devices are chip-size. If you purchase a wafer, cover it with photoresist (PR) as a protective layer to protect particles from rising on the wafer surface during cleaving. The cleaving uses a tungsten tip to make small scratches near the edge of the wafer. Do not scratch directly on the bonding surface. This is because that small scratch has a bad influence on bonding. So all samples have scratches on the back. In addition, if there is a scratch on the back side of the area where the device will be inserted, it may cause problems with the device characteristics.
The III-V die sample is 7mm x 7mm, which is suitable for handling while saving material. In the case of SOI wafer, it is designed in Chapter 2, and since the chip was received from the AMF foundary, separate cleaving is not performed. The size of the SOI chip is approximately 1cm x 1cm by filling the space allotted to us. Both SOI and III-V chips undergo solvent cleaning to remove PR as protective layer and particles. After that, O2 plasma is floated to remove the residual resist. The chip received from AMF is deposited 150nm of SiO2 as a protective layer as shown in Fig.4.3. The protective layer is removed by immersing it in Buffered Oxide Etchant (BOE) for about 30 seconds (etch rate: ~10nm/s).
This is up to step 1 of Fig.4.2.
Figure 4.3: Filmtek results. 1 Layer, shown in the lower right, 2 Layer, 3 layer and 4 layer represents the thickness of the Si substrate, BOX, Si device, protective layer, respectively. The unit is Å.
In chapter 3, the conceptual part of wafer bonding is explained in detail, and the process steps and conditions are explained in this part. Soak in piranha solution (3 H2SO4:1 H2O2 (30%)) for 2 minutes to remove organic and metallurgic contamination in SOI samples [31,32]. Then, it is immersed in hydrofluoric acid to remove the unwanted oxide layer generated during the reaction. The cap layer of InP has two layers, InP and InGaAsP, respectively. Soak in HCl (37%), 1H2SO4:8H2O2:8H2O solution for 5 seconds and 17 seconds to perform selective wet etching. Since we do Al2O3 adhesive bonding, we deposit Al2O3 on both samples by 4 nm using atomic layer deposition (ALD) equipment [40, 41].
After that, it maximizes the hydroxyl -OH groups on the surface through plasma and water treatment and leaves only the monolayer of water molecules through dehydration. Then, manually invert the prepared III-V sample and attach it to the SOI (refer to the manual bonding part in Figure 3.9). Then apply smooth pressure to hold both samples and to immobilize them while moving them to the bonding machine. The mechanical bonding was performed using SB6L bonder, and 290℃ and pressure of 1500mbar was applied for 2 hours. If the bonding was successful, there will be no debonding during substrate removal by immersion in HCl (37%). Since the thickness of the substrate is 600um, it will be stopped by the InGaAs etch stop layer after about 75 minutes. This etch stop layer is not removed at this stage, but is removed later in order to use it as a protective layer in a later process. This step is up to step 3 in Fig. 4.2. In Fig.4.4, there is a picture of the substrate removed after bonding. As mentioned above, the SOI patterning below has been produced by the AMF foundary.
Figure 4.4: Result of adhesive Al2O3 bonding, a photograph of the unetched ridge removed. In both samples, the unbonded part appeared to float or disappeared.
Hard mask patterning to form mesa structure
The contents of Steps 4 to 9 are as shown in Fig.4.2. When InP dry etching proceeds at 180℃, if a resist mask is used, it is very difficult to remove the resist because it burns. Therefore, it was decided to use a SiO2 hard mask with a fast deposition rate. 300 nm of SiO2 was deposited using plasma-enhance chemical vapor deposition (PECVD) equipment. And after applying PR (Az 5214E), lithographic patterning was done through UV exposure and development. Then, dry etch the hard mask using Metal- RIE equipment and remove the PR on it.
Figure 4.5: (a) OM image corresponding to step 8 in Figure 4.2. Resist remains and the color on the ridge appears green or pink. (b) OM image corresponding to step 9. It can be seen that the resist has been removed by looking at the blue color.
Figure 4.6: SEM image for finding etch rate for InP. We can find that the etch rate is approximately 11 nm/s.
The dry etching condition was found through Dummy InP. Etched using Metal-ICP RIE equipment, gas flow and coil power will be written down in the process flow step of the Appendix.
To preserve the thin N-contact layer, dry etching was performed up to the middle of the SCH layer, and the remaining quaternary materials were selectively wet-etched using citric acid . After this process is finished, the protective layer, SiO2, is removed. In Fig.4.7, there is the result after etching the III-V layer.
Figure 4.7: OM image after III-V etching. Until middle of SCH layer or QW layer, dry etch is carried out. After that, selective wet etching is carried out before N-contact layer.
N ohmic metal deposition
To deposit metal only in the desired area, a process called lift-off must be used. In order to properly perform lift-off, an undercut structure is required, and when this is properly formed, the metal is formed as desired without breaking. This corresponds to steps 13 to 15 in Fig.4.2. First, Az nLoF 2035, a negative resist, was selected as a resist for undercutting. In case of using the standard recipe, it was judged appropriate because the thickness of the resist was sufficiently high as 3.5um. In general, the thickness of resist must be three times higher than that of metal to proceed properly. For the metal composition, Ni/Ge/Au capable of ohmic contact with the n InP contact layer was used. After the metal is deposited, immerse in acetone and wait for about 15 minutes to remove the resist and you can see that the metal remains only in the desired area. After that, the rapid thermal annealer (RTA) process is performed for the alloy of the metal. The temperature is increased from 200°C to 420°C for 60 seconds and then heat-treated for 15 seconds. To prevent oxidation at high temperatures, the annealing is done in nitrogen atmosphere. Fig.4.8 (a) is a picture after metal deposition and lift-off process. Metal is bright yellow. Fig.4.8(b) is a picture after heat treatment is performed to form a metal alloy, and it can be seen that the color has changed compared to (a).
Figure 4.8: OM images after forming n-type ohmic metal through lift-off. (a) before annealing. (b) after annealing.
P ohmic metal deposition
It has the same steps as the previous n-ohmic metal deposition. It is the process from steps 16 to 20 in Figure 4.2. The difference from N-conact is the composition of the metal. Since the material of the P contact layer is InGaAs, Ti/Pt/Au that can make ohmic contact with the material was deposited. Another difference is that an annealing process is not required.
Figure 4.9: OM imges after lift-off for p metal.
Photo BCB (cyclotene 4022-35 bought from DOW chemical) was used to connect Ohmic metal and thick contact pad. An important point in this part is that the metal deposited with the contact pad does not break and goes well along the slope of the photo BCB. So, it is better to have a gentle slope of the photo BCB. Fig.4.10(a) is a picture of 300nm metal deposition after photo BCB patterning. As you can see here, the metal continues along the curved surface without breaking.
Figure 4.10: (a) Photo BCB test image. It can be confirmed that the metal deposited on the top has an appropriate slope and continues along the slope without breaking. (b) is an OM image patterning a real sample using photo BCB. The area marked in red is the opened area.
We can see that the part marked in red is opened in Fig.4.10(b). The area and the contact pad are connected so that current can be supplied.
Contact Pad Formation
It is the last part of the process of making a hybrid laser. The process sequence itself is the same as when depositing n and p ohmic metal. Here, Ti to increase adhesion and Au, which is connected to the tip to supply current, were deposited. If you look at Figure 4.11(a), you can see that patterning was done using negative resist. In Figure 4.11(b), Ti/Au was deposited and a contact pad was formed through the lift-off process. Through this, the production of hybrid laser device was completed.
Figure 4.11: (a) OM image patterning the part where the contact pad will rise using negative resist. (b) OM image in which the metal is deposited and the metal is left only in the desired part using the lift-off process.
Chapter 5. Characterization and discussion
The fabricated laser sample is made with Al2O3 bonding, and optical power and voltage are measured according to current through the measurement set-up in our lab. Through this, the characteristic evaluation and discussion of the laser will proceed.